LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r55369, T = 600 C, P = 17.0 kbar, cell volume = 231.15 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003168
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55369, T = 600 C, P = 17.0 kbar, cell volume = 231.15 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1371
_cell_length_b                   6.1371
_cell_length_c                   6.1371
_cell_volume                     231.148
_cell_formula_units_Z            4
_database_code_amcsd             0003257
_diffrn_ambient_pressure         1.7e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.050
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003168
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53205, T = 600 C, P = 18.1 kbar, cell volume = 230.35 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003169
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53205, T = 600 C, P = 18.1 kbar, cell volume = 230.35 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1300
_cell_length_b                   6.1300
_cell_length_c                   6.1300
_cell_volume                     230.346
_cell_formula_units_Z            4
_database_code_amcsd             0003258
_diffrn_ambient_pressure         1.81e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.057
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003169
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als3k80, T = 650 C, P = 0.0 kbar, cell volume = 257.88 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003170
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als3k80, T = 650 C, P = 0.0 kbar, cell volume = 257.88 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3651
_cell_length_b                   6.3651
_cell_length_c                   6.3651
_cell_volume                     257.879
_cell_formula_units_Z            4
_database_code_amcsd             0003259
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.837
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003170
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: als4k80, T = 650 C, P = 0.0 kbar, cell volume = 258.64 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003171
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als4k80, T = 650 C, P = 0.0 kbar, cell volume = 258.64 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3714
_cell_length_b                   6.3714
_cell_length_c                   6.3714
_cell_volume                     258.645
_cell_formula_units_Z            4
_database_code_amcsd             0003260
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.832
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003171
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55597, T = 650 C, P = 7.7 kbar, cell volume = 240.29 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003172
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55597, T = 650 C, P = 7.7 kbar, cell volume = 240.29 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2170
_cell_length_b                   6.2170
_cell_length_c                   6.2170
_cell_volume                     240.294
_cell_formula_units_Z            4
_database_code_amcsd             0003261
_diffrn_ambient_pressure         7.7e+05
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.972
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003172
Halite-sylvite thermoelasticity Sample: r53233, T = 650 C, P = 14.6 kbar, cell volume = 236.07 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003173
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53233, T = 650 C, P = 14.6 kbar, cell volume = 236.07 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1804
_cell_length_b                   6.1804
_cell_length_c                   6.1804
_cell_volume                     236.075
_cell_formula_units_Z            4
_database_code_amcsd             0003262
_diffrn_ambient_pressure         1.46e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.007
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003173
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r53217, T = 650 C, P = 18.6 kbar, cell volume = 231.94 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003174
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53217, T = 650 C, P = 18.6 kbar, cell volume = 231.94 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1441
_cell_length_b                   6.1441
_cell_length_c                   6.1441
_cell_volume                     231.940
_cell_formula_units_Z            4
_database_code_amcsd             0003263
_diffrn_ambient_pressure         1.86e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.043
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003174
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55601, T = 700 C, P = 8.0 kbar, cell volume = 241.39 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003175
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55601, T = 700 C, P = 8.0 kbar, cell volume = 241.39 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2264
_cell_length_b                   6.2264
_cell_length_c                   6.2264
_cell_volume                     241.385
_cell_formula_units_Z            4
_database_code_amcsd             0003264
_diffrn_ambient_pressure         8e+05
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    1.963
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003175
Halite-sylvite thermoelasticity Sample: r53221, T = 700 C, P = 15.6 kbar, cell volume = 235.81 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003176
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53221, T = 700 C, P = 15.6 kbar, cell volume = 235.81 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1781
_cell_length_b                   6.1781
_cell_length_c                   6.1781
_cell_volume                     235.811
_cell_formula_units_Z            4
_database_code_amcsd             0003265
_diffrn_ambient_pressure         1.56e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.009
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003176
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: r55365, T = 700 C, P = 19.0 kbar, cell volume = 231.71 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003177
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r55365, T = 700 C, P = 19.0 kbar, cell volume = 231.71 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.8Na.2)Cl
_chemical_formula_sum            'Cl K0.8 Na0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1421
_cell_length_b                   6.1421
_cell_length_c                   6.1421
_cell_volume                     231.713
_cell_formula_units_Z            4
_database_code_amcsd             0003266
_diffrn_ambient_pressure         1.9e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.045
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.8 Na.2) Cl'
_cod_database_code               9003177
_amcsd_formula_title             (K.8Na.2)Cl
Halite-sylvite thermoelasticity Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 228.78 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003178
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 228.78 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.7Na.3)Cl
_chemical_formula_sum            'Cl K0.7 Na0.3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1161
_cell_length_b                   6.1161
_cell_length_c                   6.1161
_cell_volume                     228.783
_cell_formula_units_Z            4
_database_code_amcsd             0003267
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    2.024
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.7 Na.3) Cl'
_cod_database_code               9003178
_amcsd_formula_title             (K.7Na.3)Cl
Halite-sylvite thermoelasticity Sample: als4k70, T = 500 C, P = 0.0 kbar, cell volume = 244.83 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003179
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als4k70, T = 500 C, P = 0.0 kbar, cell volume = 244.83 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.7Na.3)Cl
_chemical_formula_sum            'Cl K0.7 Na0.3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2559
_cell_length_b                   6.2559
_cell_length_c                   6.2559
_cell_volume                     244.833
_cell_formula_units_Z            4
_database_code_amcsd             0003268
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.891
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.7 Na.3) Cl'
_cod_database_code               9003179
_amcsd_formula_title             (K.7Na.3)Cl
Halite-sylvite thermoelasticity Sample: als3k70, T = 550 C, P = 0.0 kbar, cell volume = 247.23 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003180
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als3k70, T = 550 C, P = 0.0 kbar, cell volume = 247.23 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.7Na.3)Cl
_chemical_formula_sum            'Cl K0.7 Na0.3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2763
_cell_length_b                   6.2763
_cell_length_c                   6.2763
_cell_volume                     247.236
_cell_formula_units_Z            4
_database_code_amcsd             0003269
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.873
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.7 Na.3) Cl'
_cod_database_code               9003180
_amcsd_formula_title             (K.7Na.3)Cl
Halite-sylvite thermoelasticity Sample: als2k70, T = 600 C, P = 0.0 kbar, cell volume = 249.59 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003181
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als2k70, T = 600 C, P = 0.0 kbar, cell volume = 249.59 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.7Na.3)Cl
_chemical_formula_sum            'Cl K0.7 Na0.3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2962
_cell_length_b                   6.2962
_cell_length_c                   6.2962
_cell_volume                     249.595
_cell_formula_units_Z            4
_database_code_amcsd             0003270
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.855
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.7 Na.3) Cl'
_cod_database_code               9003181
_amcsd_formula_title             (K.7Na.3)Cl
Halite-sylvite thermoelasticity Sample: als1k70, T = 650 C, P = 0.0 kbar, cell volume = 252.36 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003182
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als1k70, T = 650 C, P = 0.0 kbar, cell volume = 252.36 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.7Na.3)Cl
_chemical_formula_sum            'Cl K0.7 Na0.3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.3194
_cell_length_b                   6.3194
_cell_length_c                   6.3194
_cell_volume                     252.364
_cell_formula_units_Z            4
_database_code_amcsd             0003271
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.835
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.7 Na.3) Cl'
_cod_database_code               9003182
_amcsd_formula_title             (K.7Na.3)Cl
Halite-sylvite thermoelasticity Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 221.90 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003183
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: b&w, T = 25 C, P = 0.0 kbar, cell volume = 221.90 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0541
_cell_length_b                   6.0541
_cell_length_c                   6.0541
_cell_volume                     221.896
_cell_formula_units_Z            4
_database_code_amcsd             0003272
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    2.039
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003183
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54811, T = 400 C, P = 15.0 kbar, cell volume = 216.25 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003184
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54811, T = 400 C, P = 15.0 kbar, cell volume = 216.25 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0023
_cell_length_b                   6.0023
_cell_length_c                   6.0023
_cell_volume                     216.248
_cell_formula_units_Z            4
_database_code_amcsd             0003273
_diffrn_ambient_pressure         1.5e+06
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    2.092
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003184
_amcsd_formula_title             (K.6Na.4)Cl